Download presentation

Presentation is loading. Please wait.

Published byMorris Chambers Modified about 1 year ago

1
Martin Wilson Lecture 2 slide1 'Pulsed Superconducting Magnets' CERN Academic Training May 2006 Lecture 2: Magnetization, AC Losses and Filamentary Wires magnetization from screening currents, irreversibility and hysteresis loops field errors caused by screening currents flux jumping general formulation of ac loss in terms of magnetization ac losses caused by screening currents the need for fine filaments; composite wires coupling between filaments via currents crossing the matrix

2
Martin Wilson Lecture 2 slide2 'Pulsed Superconducting Magnets' CERN Academic Training May 2006 Recap the flux penetration process B field increasing from zero field decreasing through zero plot field profile across the slab fully penetrated

3
Martin Wilson Lecture 2 slide3 'Pulsed Superconducting Magnets' CERN Academic Training May 2006 Magnetization of the Superconductor When viewed from outside the sample, the persistent currents produce a magnetic moment. As for any magnetic material, we can define a magnetization of the superconductor (magnetic moment per unit volume) NB: M is units of H I A where distributed currents flow, we must integrate over the bulk of the material For a fully penetrated superconducting slab B J J x by symmetry integrate half width B x Note: J c varies with field, so does M

4
Martin Wilson Lecture 2 slide4 'Pulsed Superconducting Magnets' CERN Academic Training May 2006 Magnetization of a Superconducting wire for cylindrical filaments the inner current boundary of screening current penetration is roughly elliptical (controversial) when fully penetrated, the magnetization is Recap: M is defined per unit volume of NbTi filament B J J J where a and d f = filament radius and diameter (compare for the slab) more commonly

5
Martin Wilson Lecture 2 slide5 'Pulsed Superconducting Magnets' CERN Academic Training May 2006 Measurement of magnetization In field, the superconductor behaves just like a magnetic material. We can plot the magnetization curve using a magnetometer. It shows hysteresis - just like iron only in this case the magnetization is both diamagnetic and paramagnetic. B M Note the minor loops, where field and therefore screening currents are reversing The magnetometer, comprising 2 balanced search coils, is placed within the bore of a superconducting solenoid. These coils are connected in series opposition and the angle of small balancing coil is adjusted such that, with nothing in the coils, there is no signal at the integrator. With a superconducting sample in one coil, the integrator measures magnetization when the solenoid field is swept up and down

6
Martin Wilson Lecture 2 slide6 'Pulsed Superconducting Magnets' CERN Academic Training May 2006 Magnetization of NbTi The induced currents produce a magnetic moment and hence a magnetization = magnetic moment per unit volume M B ext

7
Martin Wilson Lecture 2 slide7 'Pulsed Superconducting Magnets' CERN Academic Training May 2006 Reversible magnetization We have been discussing the irreversible magnetization, produced by bulk currents and thus by flux pinning. In addition, there is another component - the reversible (non hysteretic) magnetization. It is shown by all type 2 superconductors even if they have no flux pinning. In technical (strong pinning) materials however it is negligible in comparison with the irreversible component irreversible magnetization reversible magnetization

8
Martin Wilson Lecture 2 slide8 'Pulsed Superconducting Magnets' CERN Academic Training May 2006 Very fine filaments At zero external field, magnetization currents ensure that there is still a field inside the filament. Magnetization is smaller with fine filaments, so the average field within the filament is smaller. For this reason, the Jc at zero field measured on fine filament is greater than thick filaments. fine filament thick filament

9
Martin Wilson Lecture 2 slide9 'Pulsed Superconducting Magnets' CERN Academic Training May 2006 HTS magnetization Magnetization is shown by all superconducting materials. Here we see the magnetization of a high temperature superconductor. The glitches in the lower curve are flux jumps - see lecture 8

10
Martin Wilson Lecture 2 slide10 'Pulsed Superconducting Magnets' CERN Academic Training May 2006 Magnetization in superconductor field error in magnet sextupole field in the GSI FAIR prototype dipole D001 without the iron yoke, dc field in Tesla at radius 25mm measured at BNL by Animesh Jain

11
Martin Wilson Lecture 2 slide11 'Pulsed Superconducting Magnets' CERN Academic Training May 2006 Synchrotron injection synchrotron injects at low field, ramps to high field and then back down again magnetization error is worst at injection because M is largest and B is smallest, so o M / B is largest. note how quickly the magnetization changes when we start the ramp up so better to ramp up a little way, then stop to inject M B much better here! don't inject here!

12
Martin Wilson Lecture 2 slide12 'Pulsed Superconducting Magnets' CERN Academic Training May 2006 Flux penetration from another viewpoint superconductorvacuum Think of the screening currents, in terms of a gradient in fluxoid density within the superconductor. Pressure from the increasing external field pushes the fluxoids against the pinning force, and causes them to penetrate, with a characteristic gradient in fluxoid density At a certain level of field, the gradient of fluxoid density becomes unstable and collapses – a flux jump

13
Martin Wilson Lecture 2 slide13 'Pulsed Superconducting Magnets' CERN Academic Training May 2006 Flux jumping: why it happens It arises because:- magnetic field induces screening currents, flowing at critical density J c Unstable behaviour is shown by all type 2 and HT superconductors when subjected to a magnetic field BB * reduction in screening currents allows flux to move into the superconductor flux motion dissipates energy thermal diffusivity in superconductors is low, so energy dissipation causes local temperature rise critical current density falls with increasing temperature go to * QQ JcJc Cure flux jumping by making superconductor in the form of fine filaments – weakens J c Q

14
Martin Wilson Lecture 2 slide14 'Pulsed Superconducting Magnets' CERN Academic Training May 2006 Flux jumping: the numbers for NbTi typical figures for NbTi at 4.2K and 1T J c critical current density = 7.5 x 10 9 Am -2 density = 6.2 x 10 3 kg.m 3 C specific heat = 0.89 J.kg -1 K -1 c critical temperature = 9.0K Notes: least stable at low field because J c is highest instability gets worse with decreasing temperature because J c increases and C decreases criterion gives the size at which filament is just stable against infinitely small disturbances - still sensitive to moderate disturbances, eg mechanical movement better to go somewhat smaller than the limiting size in practice 50 m diameter seems to work OK Flux jumping is a solved problem so a = 33 m, ie 66 m diameter filaments criterion for stability against flux jumping a = half width of filament

15
Martin Wilson Lecture 2 slide15 'Pulsed Superconducting Magnets' CERN Academic Training May 2006 Magnetization and Losses: General so work done on magnetic material M H in general, the change in magnetic field energy (see textbooks on electromagnetism) around a closed loop, energy dissipated in material I1I1 i2i2 work done by battery to raise current in solenoid first term is change in stored energy of solenoid I 1 L 21 is the flux change produced in loop 2 so battery work done on loop a2a2

16
Martin Wilson Lecture 2 slide16 'Pulsed Superconducting Magnets' CERN Academic Training May 2006 Hysteresis Losses This is the work done on the sample Strictly speaking, we can only say it is a heat dissipation if we integrate round a loop and come back to the same place - otherwise the energy just might be stored M H Around a loop the red 'crossover' sections are complicated, but we usually approximate them as straight vertical lines (dashed) With the approximation of vertical lines at the 'turn around points' and saturation magnetization in between, the hysteresis loss per cycle is losses in Joules per m 3 and Watts per m 3 of superconductor In the (usual) situation where dH>>M, we may write the loss between two fields B 1 and B 2 as so the loss power is

17
Martin Wilson Lecture 2 slide17 'Pulsed Superconducting Magnets' CERN Academic Training May 2006 Variable current density in superconductor To evaluate need J c (B) Kim Anderson approximation loss in Joules per m 3 of superconductor recap M B B1B1 B2B2 loss for ramp up from B 1 to B 2

18
Martin Wilson Lecture 2 slide18 'Pulsed Superconducting Magnets' CERN Academic Training May 2006 The effect of transport current plot field profile across the slab B in magnets there is a transport current, coming from the power supply, in addition to magnetization currents. because the transport current 'uses up' some of the available J c the magnetization is reduced. but the loss is increased because the power supply does work and this adds to the work done by external field total loss is increased by factor (1+i 2 ) where i = I max / I c JcJc B usually not such a big factor because design for a margin in Jc most of magnet is in a field much lower than the peak

19
Martin Wilson Lecture 2 slide19 'Pulsed Superconducting Magnets' CERN Academic Training May 2006 The need for fine filaments Magnetization Flux Jumping AC Losses d as small as possible, typically 7 m critical current of a 7 m filament in 5T at 4.2K = 0.1A d f as small as possible, typically 7 m, for FAIR we are thinking of 3 m critical current of a 7 m filament in 5T at 4.2K I c = 0.1A; for a 3 m filament I c = 0.02A for NbTi d < 50 m critical current of a 50 m filament in 5T at 4.2K = 0.1A so we need multi-filamentary wires

20
Martin Wilson Lecture 2 slide20 'Pulsed Superconducting Magnets' CERN Academic Training May 2006 Fine filaments recap We can reduce M by making the superconductor as fine filaments. For ease of handling, an array of many filaments is embedded in a copper matrix Unfortunately, in changing fields, the filament are coupled together; screening currents go up the LHS filaments and return down the RHS filaments, crossing the copper at each end. In time these currents decay, but for wires ~ 100m long, the decay time is years! So the advantages of subdivision are lost

21
Martin Wilson Lecture 2 slide21 'Pulsed Superconducting Magnets' CERN Academic Training May 2006 Twisting 1 coupling may be reduced by twisting the wire coupling currents now flow along the filaments and cross over the resistive matrix every ½ twist pitch now the matrix crossing currents flow vertically, parallel to the changing field at each end of the wire, the current crosses over horizontally and then returns along the other side of the wire we assume the filaments have not reached J c and so there is no electric field along them thus the electric field due to flux change linked by the filament lies entirely on the vertical path Y thus we have a uniform electric field in the matrix where p is the twist pitch

22
Martin Wilson Lecture 2 slide22 'Pulsed Superconducting Magnets' CERN Academic Training May 2006 Twisting 2 a uniform electric field across the resistive matrix implies a uniform vertical current density J y a consideration of how this current enters and leaves the outer ring of filaments shows that there must be a linear current density g z (A/m) along the wire where where t is the transverse resistivity across the matrix and p is the twist pitch. note that, because of twist, g reverses on left hand side recap from theory of fields in magnets that a Cos current distribution around a cylinder produces a perfect dipole field inside so Ohm's law has given us the exact field needed to screen the external changing field and the internal field B i is less than the external field B e JyJy gzgz

23
Martin Wilson Lecture 2 slide23 'Pulsed Superconducting Magnets' CERN Academic Training May 2006 Twisting 3 we may define a time constant (compare with eddy currents) so that and integrate the magnetic moment of the screening currents to calculate a coupling component of magnetization provided the external field has changed by more than M cp we may take B` i ~ B` e d fb dwdw Note that the coupling magnetization is defined over the volume enclosed by the filament boundary. To define over the wire volume must multiply by a filling factor

24
Martin Wilson Lecture 2 slide24 'Pulsed Superconducting Magnets' CERN Academic Training May 2006 Twisting 4 so the total wire magnetization B M Summing the persistent current and coupling current components, we get the total magnetization of the wire. To define over the wire volume, we need a fill factor for the NbTi filaments

25
Martin Wilson Lecture 2 slide25 'Pulsed Superconducting Magnets' CERN Academic Training May 2006 Transverse resistivity JyJy J J Poor contact to filaments Good contact to filaments where is the fraction of superconductor (after J Carr) Some complications Thick copper jacket include the copper jacket as a resistance in parallel Copper core resistance in series for part of current path

26
Martin Wilson Lecture 2 slide26 'Pulsed Superconducting Magnets' CERN Academic Training May 2006 Measurement of t measure magnetization loops at different ramp rates B` plot M versus B` at chosen fields calculate t as a function of B - note the magnetoresistance

27
Martin Wilson Lecture 2 slide27 'Pulsed Superconducting Magnets' CERN Academic Training May 2006 Coupling magnetization and field errors Coupling magnetization gives a field error which adds to persistent current magnetization and is proportional to ramp rate. skew quadrupole error in Nb 3 Sn dipole which has exceptionally large coupling magnetization (University of Twente)

28
Martin Wilson Lecture 2 slide28 'Pulsed Superconducting Magnets' CERN Academic Training May 2006 Magnetization, ac losses and filamentary wires: concluding remarks magnetic fields induce persistent screening currents in superconductor - which make it look like a magnetic material with a magnetization M for the technological type 2 superconductors, the magnetization is irreversible and hysteretic, ie it depends on the history magnetization field errors in the magnet - usually the greatest source of error at injection magnetization can go unstable flux jumping quenches magnet - avoid by fine filaments - solved problem ac losses may be calculated from the area of the magnetization hysteresis loop (remember this is only the work done by the external field, transport current loss is extra) magnetization is proportional to filament diameter, so can reduce these problems by making fine filaments - typically 50 m for flux jumping and m for losses and field quality practical conductors are made in the form of composite wires with superconducting filaments embedded in a matrix of copper in changing fields the filaments are coupled together through the matrix, thereby losing the benefit of subdivision twisting the composite wire reduces coupling coupling time constant depends on twist pitch and effective transverse resistivity, which is a function of contact resistance and geometry

Similar presentations

© 2017 SlidePlayer.com Inc.

All rights reserved.

Ads by Google